Heterometallic molecular precursors for a lithium-iron oxide material: synthesis, solid state structure, solution and gas-phase behaviour, and thermal decomposition.
Han, Haixiang; Wei, Zheng; Barry, Matthew C.; Filatov, Alexander S.; Dikarev, Evgeny V.; Dalton transactions (Cambridge, England : 2003) 46 (2017) 5644–5649; doi:10.1039/c6dt04602a

data_7041687
_publ_section_title
;
 Heterometallic molecular precursors for a lithium-iron oxide material:
 synthesis, solid state structure, solution and gas-phase behaviour, and
 thermal decomposition.
;
_journal_issue                   17
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              5644
_journal_page_last               5649
_journal_paper_doi               10.1039/c6dt04602a
_journal_volume                  46
_journal_year                    2017
_chemical_formula_moiety         'C48 H60 F18 Fe2 Li2 O12'
_chemical_formula_sum            'C48 H60 F18 Fe2 Li2 O12'
_chemical_formula_weight         1296.54
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2016-11-21 deposited with the CCDC.
2017-01-13 downloaded from the CCDC.
;
_cell_angle_alpha                91.399(2)
_cell_angle_beta                 113.519(2)
_cell_angle_gamma                100.038(2)
_cell_formula_units_Z            1
_cell_length_a                   11.3877(11)
_cell_length_b                   11.8362(11)
_cell_length_c                   11.9720(11)
_cell_measurement_reflns_used    9936
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      28.68
_cell_measurement_theta_min      2.87
_cell_volume                     1449.1(2)
_computing_cell_refinement       'SAINT V.8.27 (Bruker AXS Inc., 2012)'
_computing_data_collection       'APEX2 v.2016.1-0 (Bruker AXS Inc., 2016)'
_computing_data_reduction        'SAINT V.8.27 (Bruker AXS Inc., 2012)'
_computing_molecular_graphics    'SHELXTL Ver. 6.14'
_computing_publication_material  'SHELXTL Ver. 6.14'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker D8 Venture PHOTON 100 CMOS'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0437
_diffrn_reflns_av_sigmaI/netI    0.0274
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            70343
_diffrn_reflns_theta_full        28.69
_diffrn_reflns_theta_max         28.69
_diffrn_reflns_theta_min         3.24
_exptl_absorpt_coefficient_mu    0.614
_exptl_absorpt_correction_T_max  0.9526
_exptl_absorpt_correction_T_min  0.8976
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS V2012/1 (Bruker AXS Inc.)
;
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.486
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    none
_exptl_crystal_description       needle
_exptl_crystal_F_000             664
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_refine_diff_density_max         0.784
_refine_diff_density_min         -0.641
_refine_diff_density_rms         0.085
_refine_ls_extinction_coef       noref
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     387
_refine_ls_number_reflns         7452
_refine_ls_number_restraints     18
_refine_ls_restrained_S_all      1.073
_refine_ls_R_factor_all          0.0637
_refine_ls_R_factor_gt           0.0487
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0463P)^2^+2.5546P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1104
_refine_ls_wR_factor_ref         0.1189
_reflns_number_gt                6219
_reflns_number_total             7452
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c6dt04602a2.cif
_cod_data_source_block           LiFeptac3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7041683--7041687.cif.
;
_cod_database_code               7041687